The advancement of nanotechnology provides opportunities for fabrication of nanoscale materials and higher performance devices using nanomaterials with high precision. Currently, various nanomaterials and nanostructures in the range of 1 to 100 nm have been produced by chemical and physical methods. Among various nanostructured materials, one-dimensional (1D) materials, such as nanowires, nanotubes, nanorods, and nanobelts, have potential applications in nanoscale electronics (Cui & Lieber, 2001), optoelectronics (Duan et al., 2001), photonics (Gudiksen et al., 2002; Huang et al., 2001), sensors ( Cui et al., 2001 ), and solar cells (Law et al., 2005) due to their unique electrical, chemical, and optical properties (Li et al., 2006; Thelander et al., 2006; Wang et al., 2008). Nanowires are useful in chemical or biological sensors for detecting single molecules because they have a high surface-to-volume ratio and a highly sensitive 1D nanostructure that gives rise to large conductivity change associated with binding molecules (Cui et al., 2001; Ramanathan et al., 2005).
Conducting polymers, such as polypyrrole, polyaniline, polythiophene, and their derivatives, are promising materials for synthesis of nanostructured materials and devices (Langea et al., 2008; Malinauskas et al., 2005). Compared with other materials, conducting polymers have some unique electrical, chemical, and optical properties because of their conjugated structures, and they are easily synthesized using chemical or electrochemical synthetic methods at room temperatures with low cost (Aleshin, 2006; Briseno et al., 2008; Guimard et al., 2007; Xia et al., 2010). Conducting polymers have electrical and optical properties similar to those of metals and semiconductors, while maintaining the flexibility and properties commonly associated with conventional polymer substances (Dai et al., 2002; Heeger, 2002; Shirakawa, 2002). For example, the electrical conductivity of these polymers can be adjusted from an insulator to traditional metals by varying the species and concentrations of doping ions. Undoped conducting polymers with conductivities of 10-10 to 10-5 S cm-1 can be changed into semiconducting or metallic materials with conductivities of 1 to 104 S cm-1 through a chemical or electrochemical doping process (MacDiarmid, 2002). Also, optical absorption bands and mechanical volume of conducting polymers can be changed by entrapped doping ions. Therefore, they have been used for various applications such as electronic devices (Hashizume, 2006), optoelectronic devices (Noy et al., 2002), actuators (Berdichevsky & Lo, 2006), transistors (Alam et al., 2005), and chemical sensors (Bangar et al., 2009; García-Aljaro et al., 2010).
In recent years, 1D conducting polymer nanostructures have been demonstrated to have improved performance with low dimensionality. Many different fabrication methods have been applied to making conducting polymer nanowires. These methods include e-beam lithography, focused ion-beam etching, dip-pen lithography, electro-spinning, DNA scaffolding, mechanical break junction, hydrodynamically focused stream, and nanopore template. In this chapter, we will introduce various fabrication methods for conducting polymer nanowires. This chapter is describes four methods: the template method, electro-spinning method, nanolithography method, and microfluidic method.
2. Template method
The template method has been widely used to fabricate 1D conducting polymer nanostructures such as nanowires and nanotubes because of its simplicity, versatility, and controllability (Cho & Lee, 2007; Tran et al., 2009). Generally, the template method has been classified into a hard-template method, which uses a nanopore film such as anodic aluminium oxide (AAO), and a soft-template method, which uses the self-assembly ability of molecules such as surfactants and DNA.
2.1. Hard template
In the early 1990s, Martin and co-workers introduced the fabrication of various conducting polymer nanowires such as polypyrrole, polyaniline, poly(3-methylthiophene), and polyacetylene using a nanoporous polycarbonate and aluminium oxide template. Figure 1 shows SEM images of these nanowires and their templates (Cai et al., 1991; Cai & Martin, 1989; Liang & Martin, 1990; Martin et al., 1993; Parthasarathy & Martin,1994). These polymers are electrochemically or chemically polymerized from corresponding monomers using an oxidizing agent (Martin, 1994). This process is composed of simple steps: 1) fill nanopores of the membrane with monomers, 2) polymerize the monomers inside the nanopores, and 3) remove the nanopore template to obtain pure polymers (Tran et al., 2009).
Later, a method was sought to control the composition or properties of conducting polymer nanowires. Jèrôm et al. (1999) fabricated high-aspect-ratio polypyrrole nanowires 600 nm in diameter and 300 μm in length using a two-step electrochemical method. After electro-polymerization of polyacrylate films on the cathode, polypyrrole was synthesized by chronopotentiometry under a constant current of 0.5 mA/cm2 in a dimethylformamide solution. Fu et al. (2001) synthesized polythiophene nanowires on flexible gold film by electro-polymerization of thiophene in boron trifluoride diethyl etherate solution using an alumina membrane. The length and diameter of various conducting polymer nanowires synthesized using AAO templates can be controlled by polymerization time and current (Joo et al., 2005; 2003; Park et al., 2005; Xiao et al., 2007). The electrical properties of conducting polymers were controlled through various synthetic conditions, such as doping level, dopant, and template-dissolving solvents (Kim et al., 2005). Li et al. (2001; 2002) copolymerized pyrrole/aniline and pyrrole/thiophene composite nanowires using AAO. The diameter and length could be controlled by the shape of the nanopores of the AAO membrane. The composition of nanowires can be controlled by electrochemical polymerization potentials, and it can be estimated indirectly using cyclic voltammetry and IR spectroscopy. Wang et al. (2005) fabricated polypyrrole/carbon nanotube composite nanowires to improve the electrical and mechanical properties of polymers. Electro-polymerization of polypyrrole was achieved using carboxylated CNT (carbon-nanotube) dopants in nanoporous alumina membranes. Figure 2 shows a SEM image of various conducting polymer nanowires using a hard template.
The fabrication method using a hard template provides a straightforward system to synthesize conducting polymer nanowires. The diameter and length of nanowires are controllable by adjusting the pore size, thickness of the membrane, and polymerization conditions. On the other hand, this method requires a post-synthesis task to obtain pure polymer nanowires. In some cases, polymer nanowires can be destroyed or damaged because the template removal process entails harsh conditions. AAO, one of the most widely used nano templates, is a representative example.
2.2. Soft template
The soft-template method which is also called the self-assembly method typically uses surfactants or DNA as templates. This method has the advantage of a simple fabrication process, and the template removal process is achieved under mild conditions or is not required. Thus, it is possible to avoid the damage that occurs during the removal of a hard template.
Surfactants offer a representative soft template because of their self-assembly ability. Wan et al. (1998) accidentally discovered that polyaniline nanowires could be synthesized by
DNA molecules also provide attractive soft templates for nanowire fabrication because they are chemically robust and are able to react with monomers without obvious structural requirements or functional group adjacency (Moon et al., 2010; Xia et al., 2010). Ma et al. (2004) immobilized stretched double stranded λ-DNA on a thermally oxidized silicon chip using the molecular combining method. The DNA templates were incubated in aniline monomer solutions (19 mM, pH = 4.0), and the phosphate groups in the DNA templates and protonated aniline monomers were organized by electrostatic interactions. The aligned aniline monomers were enzymatically polymerized by adding horseradish peroxidase and H2O2 successively. Figure 4 shows the fabrication process of polyaniline/DNA nanowires introduced by Ma et al. (2004). Polypyrrole nanowires were chemically polymerized on mica with FeCl3 oxidant using DNA as a template by Dong et al. (2007). Moon et al. (2010) also chemically polymerized polypyrrole nanowires using DNA as a template on a (3-aminopropyl)triethoxysilane modified silicon wafer with ammonium persulfate as an oxidant. Hassanien et al. (2010) reported that polyindole nanowires were synthesized on a λ-DNA template by chemical oxidation of indole using FeCl3 as an oxidant. Figure 3 shows AFM images of conducting polymer nanowires using DNA as a template.
Electro-spinning has been recognized as one of the most efficient techniques for the fabrication of micro- or nanoscale polymer fibers. Electro-spinning occurs with the development of a jet when the repulsion forces of a charged solution overcome the surface tension of the solution under a high electrostatic field. When the jet solidifies, polymer nanofibers remain (Huang et al., 2003; Reneker & Chun, 1996).
In recent years, it has been reported that various polymers including conducting polymers have been successfully electrospun into polymer nanofibers. MacDiarmid et al. (2001) reported fabrication of polyanlin nanowires with sub-100 nm diameters doped with
Electro-spinning is a very effective method for fabrication of conducting polymer nanowires; however, it is limited in its application for various electronic devices owing to the nonwoven fiber shape and the difficulty of controlling positioning. Kameoka et al. (2003) presented a method for the controlled deposition of oriented nanowires with the rotation of collectors using a chopper motor. Although this method is not limited by nonwoven shape, it still has limits compared with other methods.
Nanowire sensors are among the most promising applications because of their impressive sensitivities to detect nanomolar concentrations of DNA (Kemp et al., 2007) and ~10 fM concentrations of micro-RNAs (Fan et al., 2007). To detect such small concentrations of analytes, electrode–wire–electrode assemblies are required (Thapa et al., 2009). The aforementioned fabrication methods can yield uniform nanowires with a high throughput, but they require the elaborate post-synthesis task of positioning the nanowires with the desired precision and electrical contact properties to create one-dimensional nanostructures. The simplest nanowire-positioning technique uses dielectrophoresis (Dan et al., 2007) and self-assembly at the air/water interface (Xu et al., 2009). On the other hand, nanolithography makes it possible to synthesize the nanowires in the desired position. This method allows simultaneous synthesis and positioning of the conducting polymer nanowires.
4.1. Dip-pen nanolithography
Dip-pen nanolithography (DPN), in which an atomic force microscope (AFM) tip transfers alkane thiol to a gold surface, is one of the best-known nanolithography techniques. It is possible to directly write on the desired position without a photomask using an AFM tip as a "pen" (Piner et al., 1999). Lim & Mirkin (2002) synthesized conducting polymer nanowires using DPN using self-doped sulfonated polyaniline (SPAN) and doped polypyrrole as "ink" on a positively charged surface using 2% (trimethoxysilyl)propyldiethylenetriamine (DETA) (Fig. 7). Because SPAN and doped polypyrrole are negatively charged, an electrostatic
interaction makes it possible to draw conducting polymer nanowires using DPN. It is possible to control the width of the polymer pattern owing to the linear dependence on the root of contact time (Fig. 8). Maynor et al. (2002) reported the PEDOT line deposition on an anodic silicon surface simultaneous with oxidation. Fig. 9 shows conducting polymer lines drawn using DPN.
4.2. e-beam lithography
Yun et al. (2004) and Ramanathan et al. (2004) reported a method of fabricating an array of individually addressable conducting polymer nanowires using e-beam lithography. Figure 10 shows schematic diagram and SEM image of a conducting polymer nanowireusing e-beam lithography. They patterned nano channel arrays for the electro-deposition of wires between the electrodes using e-beam lithography. Monomer solutions, such as pyrrole (0.06 M in 0.01 M KCl) or aniline (0.1 M in 0.01 M KCl), were placed on the nanochannel between the electrodes, and the electro-polymerization was generated by applying an electric current. Because the electro-polymerization occurs only in nanochannels, it is possible to control various properties of the nanowires such as dimensions, position, alignment, and chemical composition. This technique is similar to the hard-template method in that nanowire synthesis occurs in nanochannels. The hard-template method is suitable for fabricating nanowires with high density within definite area, whereas e-beam lithography is suitable for fabricating a single nanowire at a desired position, such as in an electrode–wire–electrode structure.
Conducting-polymer fabrication methods based on nanolithography such as Dip-pen and e-beam are attractive because it is possible to synthesize conducting polymers in a desired position to avoid the post-synthesis positioning task. However, they have obvious limitations, such as high cost and low yield, which are characteristic of nanolithgraphy.
5. Fabrication using microfluidics
Nanolithography is an attractive technique because nanowires with a diameter of several tens of nanometers can be reproducibly obtained at a desired position. However, nanolithography is not suitable for commercialization because of a low yield and high cost. Fabrication methods using microfluidics make it possible not only to synthesize nanowires in the desired position but also to produce nanowires at a low cost. Limitations such as reproducibility and a slightly larger diameter of nanowires still exist.
5.1. Hydrodynamic focusing
Hou et al. (2008) introduced a fabrication method that uses the characteristics of laminar flow in micro-channels. In the microfluidic system, a low Reynolds number causes a small diffusion layer between miscible liquids. The microfluidic device reported by Hou et al. was made up of polydimethylsiloxane micro-channels and a platinum electrode array on a glass substrate (Fig. 11a). The pyrrole solution (0.1 M pyrrole, 0.1 M LiClO, and 1.0 mM HCl) was inserted into the centre of the microchannel at a constant flow rate, while the distilled water comprised a sheath flow at a variable flow rate. Figure 11b shows the fluorescence images of hydrodynamically focused pyrrole solutions containing a fluorescent component (10 nM 5-carboxyfluorescein). The two-step sheath flow created a compressed monomer layer in the centre of the microchannel, and this layer flowed across the platinum electrode arrays. The thickness of the compressed layer was controlled by changing the flow rate of the sheath flow. Applying constant current between the electrodes, a conducting polymer micropattern was electropolymerized in a focused monomer stream as a dynamic template (Fig. 11c). The width of the polypyrrole wire could be controlled by the width of the focused stream, the gap between electrodes, and the electro-polymerization time.
Strictly speaking, it is hard produce a nanowire because the smallest published width of a conducting polymer wire is just 1 μm. However, this technique shows the potential to fabricate conducting polymer nanowires by controlling the polymerization conditions. Moreover, the conducting polymer can be synthesized with low cost and high throughput by applying an electric field to the desired electrodes. For this reason, we introduce a hydrodynamic focused fabrication method in this chapter.
Choi et al. (2009) electrochemically synthesized CNT–conducting polymer nanowires using dielectrophoresis. CNTs and monomer precursors were gathered between the electrodes where the electric-field gradient is greater due to their higher conductivity compared with the surrounding medium (Fig. 12a). After the suspension was partially removed, the remaining suspension was compressed, and it formed a concave meniscus with evaporation due to surface tension (Fig. 12b). As a result, the electric current was concentrated through the compressed CNTs and monomers. Gathered CNTs generated dynamic templates for electro-polymerization of conducting polymer nanowires. Because nanowires are synthesized between the electrodes to which an electric field is applied, it is possible to individually address a conducting polymer nanowire array to a single chip. Figures 13 shows SEM images of various conducting polymer nanowires on a single chip. These CNT– conducting polymer nanowires are a few hundred nanometers in diameter and a few micrometers in length.
This chapter has provided a brief overview of the methods of fabricating conducting polymer nanowires. Since Martin and co-workers first reported conducting polymer nanowires, which were synthesized using nanopore templates, various fabrication methods have been developed. Template methods consist of a simple synthesis process to produce nanowires and can control the size of nanowires by adjusting the nanopore of templates. Electro-spinning is a method to obtain a mass quantity of nanowires with a nonwoven fiber structure using a high electric field. Template and electro-spinning methods are possible options to fabricate nanowires with high yield and low cost; however, they require a post-synthesis task to address the desired nanowire position in some applications that need a single nanowire. In the case of nanolithography, wire synthesis and positioning occur simultaneously because polymerization occurs according to the nano pattern drawn by e-beam or dip-pen nanolithography. This method can control the properties of each individual nanowire; however, it is expensive, and a long production time is required to synthesize a large quantity of nanowires. In the case of the method using microfluidics, polymerization occurs in compressed monomer precursors through hydrodynamic focusing or dielectrophoresis. This method allows for the control of the properties of each individual nanowire in a similar manner to nanolithography. Compared with nanolithography, microfluidics has advantages such as low cost and high yield along with limitations such as size control and reproducibility.
Although many techniques have been developed to fabricate conducting polymer nanowires, still some limitations remain such as size control, low yield, high cost, or long production time due to post-synthesis tasks. Further research is needed to overcome these limitations and develop applications for commercialization.
Alam M. M. Wang J. Guo Y. Lee S. P. Tseng H. R. 2005Electrolyte gated transistors based on conducting polymer nanowire junction arrays,
Aleshin A. N. 2006Polymer nanofibers and nanotubes: Charge transport and device applications, Adv. Mater. 18 17 27.
Bangar M. A. Shirale D. J. Chen W. Myung N. V. Mulchandani A. 2009Single conducting polymer nanowire chemiresistive label-free immunosensor for cancer biomarker, Anal. Chem. 81 6 2168 2175.
Berdichevsky Y. Lo Y. H. 2006Polypyrrole nanowire actuators, Adv. Mater. 18 122 125.
Briseno A. L. Mannsfeld S. C. B. Jenekhe S. A. Bao Z. Xia Y. 2008Introducing organic nanowire transistors, Mater. Today 11 4 38 47.
Cai Z. Lei J. Liang W. Menon V. Martin C. R. 1991Molecular and supermolecular origins of enhanced electric conductivity in template-synthesized polyheterocyclic fibrils. 1. Supermolecular effects, Chem. Mater. 3 5 960 967.
Cai Z. Martin C. R. 1989Electronically conductive polymer fibers with mesoscopic diameters show enhanced electronic conductivities, J. Am. Chem. Soc. 111 11 4138 4139.
Cho S. I. Lee S. B. 2007Fast electrochemistry of conductive polymer nanotubes: Synthesis, mechanism, and application, Accounts Chem. Res. 41 6 699 707.
Choi J. Lee J. Choi J. Jung D. Shim S. E. 2010Electrospun PEDOT:PSS/PVP nanofibers as the chemiresistor in chemical vapour sensing, Synth. Met. 160 1415 1421.
Choi W. An T. Lim G. 2009Fabrication of conducting polymer nanowire sensor array,
Chronakis I. S. Grapenson S. Jakob A. 2006Conductive polypyrrole nanofibers vis electrospinning: Electrical and morphological properties, Polymer 47 5 1597 1603.
Cui Y. Lieber C. M. 2001Functional nanoscale electronic devices assembled using silicon nanowire building blocks, Science 291 5505 851 853.
Cui Y. Wei Q. Park H. Lieber C. M. 2001Nanowire nanosensors for highly sensitive and selective detection of biological and chemical species, Science 293 5533 1289 1292.
Dai L. Soundarrajan P. Kim T. 2002Sensors and sensor arrays based on conjugated polymers and carbon nanotubes, Pure Appl. chem. 74 9 1753 1772.
Dan Y. Cao Y. Mallouk T. E. Johnson A. T. Evoy S. 2007Dielectrophoretically assembled polymer nanowires for gas sensinig, Sens. Actuator A 125 55 59.
Dong L. Hollis T. Fishwick S. Connolly B. A. Wright N. G. Horrocks B. R. Houlton A. 2007Synthesis, manipulation and conductivity of supramolecular polymer nanowires, Chem. Eur. J. 13 3 822 828.
Duan X. Huang Y. Cui Y. Wang J. Lieber C. M. 2001Indium phosphide nanowires as building blocks for nanoscale electronic and optoelectronic devices, Nature 409 6816 66 69.
Fan Y. Chen X. Trigg A. D. hang Tung. C. Kong J. Gao Z. 2007Detection of microRNAs using target-guided formation of conducting polymer nanowires in nanogaps, J. Am. Chem. Soc. 129 17 5437 5443.
Fu M. Zhu Y. Tan R. Shi G. 2001Aligned polythiophene micro- and nanotubules, Adv. Mater. 13 1874 1877.
García-Aljaro C. Bangar M. A. Baldrich E. noz F. J. M. Mulchandani A. 2010Conducting polymer nanowire-based chemiresistive biosensor for the detection of bacterial spores, Biosens. Bioelectron. 25 2309 2312.
Gudiksen M. S. Lauhon L. J. Wang J. Smith D. C. Lieber C. M. 2002Growth of nanowire superlattice structures for nanoscale photonics and electronics, Nature 415 6872 617 620.
Guimard N. K. Gomez N. Schmidt C. E. 2007Conducting polymers in biomedical engineering, Prog. Polym. Sci. 32 876 921.
Hashizume T. 2006Propertiy of individual conducting-polymer nanowires: conductance and fet devices,
Hassanien R. Al-Hinai M. Al-Said S. A. F. Little R. Ŝiller L. Wright N. G. Houlton A. Horrocks B. R. 2010Preparation and characterization of conductive and phhotoluminescent dna-templated polyindole nanowires, ACS Nano 4 4 2149 2159.
Heeger A. J. 2002Semiconducting and metallic polymers: the forth generation of polymeric metals, Synth. Met. 125 23 42.
Hou S. Wang S. Yu Z. Zhu N. Liu K. Sun J. Lin W. Y. Shen C. F. Fang X. Tseng H. R. 2008A hydrodynamically focused stream as a dynamic template for site-specific electrochemical micropatterning of conducting polymers, Angew. Chem. 120 6 1088 1091.
Huang M. H. Mao S. Feick H. Yan H. Wu Y. Kind H. Weber E. Russo R. Yang P. 2001Room-temperature ultraviolet nanowire nanolasers, Science 292 5523 1897 1899.
Huang Z. M. Zhang Y. Z. Kotaki M. Ramakrishna S. 2003A review on polymer nanofibers by electrospinning and their applications in nanocomposites, Compos. Sci. Technol. 63 15 2223 2253.
Jèrôme C. Labaye D. Bodart I. Jèrôme R. 1999Electrosynthesis of polyacrylic/polypyrrole compostes: formation of polypyttole wires, Synth. Met. 101 3 4.
Joo J. Kim B. H. Parka D. H. Kim H. S. Seo D. S. Shim J. H. Lee S. J. Ryu K. S. Kim K. Jin J. I. Lee T. J. Lee C. 2005Fabrication and applications of conducting polymer nanotube, nanowire, nanohole, and double wall nanotube, Synth. Met. 153 313 316.
Joo J. Park K. T. Kim B. H. Kim M. S. Lee S. Y. Jeong C. K. Lee J. K. Park D. H. Yi W. K. Lee S. H. Ryu K. S. 2003Conducting polymer nanotube and nanowire synthesized by using nanoporous template: Synthesis, characteristics, and application,
Ju Y. W. Park J. H. Jung H. R. Lee W. J. 2007Electrochemical properties of polypyrrole/sulfonated SEBS composite nanofibers prepared by electrospinning, Electrochim. Acta 52 14 4841 4847.
Kameoka J. Orth R. Yang Y. Czaplewski D. Mathers R. Coates G. W. Craighead H. G. 2003A scanning tip electrospinning source for deposition of oriented nanofibers,
Kemp N. T. Mc Grouther D. Cochrane J. W. Newbury R. 2007Bridging the gap: Polymer nanowire devices, Adv. Mater. 19 18 2634 2638.
Kim B. H. Park D. H. Joo J. Yu S. Lee S. H. 2005Synthesis, characteristics, and field emission of doped and de-doped polypyrrole, polyaniline, poly(3,4-ethylenedioxythiophene) nanotubes and nanowires, Synth. Met. 150 279 284.
Laforgue A. Robitaille L. 2010Production of conductive PEDOT nanofibers by the combination of electrospinning and vapor-phase polymerization, Macromolecules 43 9 4194 4200.
Langea U. Roznyatovskaya N. V. Mirsky V. M. 2008Conducting polymers in chemical sensors and arrays, Anal. Chim. Acta 614 1 1 26.
Law M. Greene L. E. Johnson J. C. Saykally R. Yang P. 2005Nanowire dye-sensitized solar cells, Nat. Mater. 4 6 455 459.
Li G. Zhang Z. 2004Synthesis of dendritic polyaniline nanofibers in a surfactant gel, Macromolecules 37 2683 2685.
Li X. Lu M. Li H. 2001Preparation and characterization of pyrrole/aniline copolymer nanofibrils using the template-synthesis method, J. Appl. Polym. Sci. 81 3002 3007.
Li X. Lu M. Li H. 2002Electrochemical copolymerization of pyrrole and thiophene nanofibrils using template-synthesis method, J. Appl. Polym. Sci. 86 2403 2407.
Li Y. Qian F. Xiang J. Lieber C. M. 2006Nanowire electronic and optoelectronic devices, Mater. Today 9 10 18 27.
Liang W. Martin C. 19901990. Template-synthesized polyacetylene fibrils show enhanced supermolecular order, J. Am. Chem. Soc. 112 26 9666 9668.
Lim J. H. Mirkin C. A. 2002Electrostatically driven dip-pen nanolithography of conducting polymers, Adv. Mater. 14 20 1474 1477.
Ma Y. Zhang J. Zhang G. He H. 2004Polyaniline nanowires on Si surfaces fabricated with dna templates, J. Am. Chem. Soc. 126 22 7097 7101.
Mac Diarmid. A. G. 2002Synthetic metals: a novel role for organic polymers, Synth. Met. 125 11 22.
Mac Diarmid. A. G. Jones W. E. Norris I. D. Gao J. Johnson A. T. Pinto N. J. Hone J. Han B. Ko F. K. Okuzaki H. Llaguno M. 2001Electrostatically-generated nanofibers of electronic polymers, Synth. Met. 119 27 30.
Malinauskas A. Malinauskiene J. Ramanavičius A. 2005Conducting polymer-based nanostructurized materials: Electrochemical aspects,
Martin C. R. 1994Nanomaterials: A membraine-based synthetic approach, Science 266 1961 1966.
Martin C. R. Parthasarathy R. Menon V. 1993Template synthesis of electronically conductive polymers- A new route for achieving higher electronic conductivities, Synth. Met. 55 1165 1170.
Maynor B. W. Filocamo S. F. Grinstaff M. W. Liu J. 2002Direct-writing of polymer nanostructures: Poly(thiophene) nanowires on semiconducting and insulating surfaces, J. Am. Chem. Soc. 124 4 522 523.
Moon H. K. Kim H. J. Kim N. H. Roh Y. 2010Fabrication of highly uniform conductive polypyrrole nanowires with dna template, J. Nanosci. Nanotechnol. 10 3180 3184.
Norris I. D. Shaker M. M. Ko F. K. Mac Diarmid. A. G. 2000Electrostatic fabrication of ultrafine conducting fibers: polyaniline/polyethylene oxide blends, Synth. Met. 114 109 114.
Noy A. Miller A. E. Klare J. E. Weeks B. L. Woods B. W. De Yoreo J. J. 2002Fabrication of luminescent nanostructures and polymer nanowires using dip-pen nanolithography, Nano Lett. 2 2 109 112.
Park D. H. Kim B. H. Jang M. K. ans S. J. Lee K. Y. B. Joo J. 2005Synthesis and characterization of polythiophene and poly (3-methylthiophene) nanotubes and nanowires, Synth. Met. 153 341 344.
Parthasarathy R. V. Martin C. R. 1994Template-synthesized polyaniline microtubules, Chem. Mater. 6 1627 1632.
Piner R. D. Zhu J. Xu F. Hong S. Markin C. A. 1999"Dip-pen" nanolithography, Science 283 29 661 662.
Ramanathan K. Bangar M. A. Yun M. Chen W. Mulchandani A. Myung N. V. 2004Individually addressable conducting polymer nanowires array, Nano Lett. 4 7 1237 1239.
Ramanathan K. Bangar M. A. Yun M. Chen W. Myung N. V. Mulchandani A. 2005Bioaffinity sensing using biologically functionalized conducting-polymer nanowire, J. Am. Chem. Soc. 127 2 496 497.
Reneker D. H. Chun I. 1996Nanometre diameter fibres of polymer, produced by electrospinning, Nanotechnology 7 216 223.
Shirakawa H. 2002The discovery of polyacetylene film the dawining of an era of conducting polymers, Synth. Met. 125 3 10.
Thapa P. S. Yu D. J. Wicksted J. P. Hadwiger J. A. Barisci J. N. Baughman R. H. Flanders B. N. 2009Directional growth of polypyrrole and polythiophene wires,
Thelander C. Agarwal P. Brongersman S. Eymery J. Feiner L. F. Forchel A. Scheffler M. Riess W. Ohlsson B. J. Gösele U. Samuelson L. 2006Nanowire-based one-dimensional electronics, Mater. Today 9 10 28 35.
Tran H. D. Li D. Kaner R. B. 2009One-dimensional conducting polymer nanostructures: Bulk synthesis and applications, Adv. Mater. 21 1487 1499.
Wan M. X. Shen Y. Q. Huang J. 1998Chinese patent 981099165.
Wang J. Dai J. Yarlagadda T. 2005Carbon nanotube-conducting-polymer composite nanowires, Langmuir 21 1 9 12.
Wang N. Cai Y. Zhang R. Q. 2008Growth of nanowires, Mater. Sci. Eng. R-Rep. 60 1 51.
Wei Z. Zhang Z. Wan M. 2002Formation mechanism of self-assembled polyaniline micro/nanotubes, Langmuir 18 917 921.
Xia L. Wei Z. Wan M. 2010Conducting polymer nanostructures and their application in biosensors, J. Colloid Interface Sci. 341 1 11.
Xiao R. Cho S. I. Liu R. Lee S. B. 2007Controlled electrochemical synthesis of conductive polymer nanotube structures, J. Am. Chem. Soc. 129 4483 4489.
Xu J. Jiang Y. Yang Y. Yu J. 2009Self-assembly of conducting polymer nanowires at air-water interface and its application for gas sensors, Mater. Sci. Eng. B 157 87 92.
Yun M. Myung N. V. Vasquez R. P. Lee C. Menke E. Penner R. M. 2004Electrochemically grown wires for individually addressable sensor arrays, Nano Lett. 4 3 419 422.
Zhang X. Zhang J. Liu Z. Robinson C. 2004Inorganic/organic mesostructure directed synthesis of wire/ribbon-like polypyrrole nanostructures,
Zhang X. Zhang J. Song W. Kiu Z. 2006Controllable synthesis of conducting polypyrrole nanostructures, J. Phys. Chem. B. 110 3 1158 1165.
Zhou Y. Freitag M. Hone J. Staii C. Johnson A. T. Pinto N. J. Mac Diarmid. A. G. 2003Fabrication and electrical characterization of polyaniline-based nanofibers with diameter below 30, Appl. Phys. Lett. 83 18 3800 3802.